A Guide to Rotational Molding
Figure 1. Various rotomolded toys
A Guide to Rotational MoldingIntroductionRotational molding also referred to as rotomolding or rotational casting is one of the fastest growing plastics processing methods today. Its easy to see why. Rotational molding techniques coupled with Microthene polyolefin powders from Equistar Chemicals can be used to make hollow items of any size, open or closed, and of any desired shape. In recent years, rotomolding techniques have been developed extensively. On the production line, this process can now compete with or outperform blow molding, injection molding and thermoforming. In many cases, pieces virtually impossible to fabricate by any other processes can be produced by rotomolding. Rotational molding was first developed early in the 20th century. But it wasnt until the early 1960s, when Equistar Chemicals replaced vinyl plastisol resins with polyolefin resins, that rotomolding gained wide acceptance. Within a few years, the development of low and high density polyethylene specifically designed for rotomolding enabled rotational molders to enter markets where vinyl parts and processes could not compete. In the early 1970s, crosslinkable and modified polyethylene grades made their way into the rotational molding market. These new resins again opened up more new market areas, especially production of large tanks. Linear low density polyethylene for rotomolding was developed in the late 1970s, while the 1980s brought a surge of non-polyethylene resins, including nylon, polypropylene and polycarbonate for rotomolding.
Figure 2. Smaller storage bins and refuse containers are also rotomolded
Rotomolding is differentThe main difference between rotational molding and other plastics molding techniques, such as blow and injection molding, are as follows: resin powder is used instead of pellets; the resin melts in the molds instead of being forced under pressure into the molds in a molten state; the mold has a biaxial rotation; rotomolding molds are less expensive because of their simplicity; and operating pressures are relatively low, allowing molds to be made from less expensive materials. In rotational molding, rigid, resilient hollow bodies are formed by powdered plastic material in heated molds, which are rotated simultaneously in two planes perpendicular to each other. The plastic particles make contact and melt on the inner surfaces of the hot molds and fuse in layers until all the powder is fused and the desired end product and wall thickness is obtained. The wall thickness is controlled by the amount of powder placed in the mold. Rotationally molded pieces are stress-free except for slight shrinkage forces because the pieces are produced without any external pressure. Additionally, there is practically no scrap in rotational molding. The uniformity of wall thickness can be maintained to within 10 percent, which is better than that normally possible with the blow molding process. Wall thicknesses can range from 1/32 inch to 1 inch (0.8mm to 25mm). Most resins used in rotational molding are powders ground to 35 mesh and ranging in diameter from 74 microns to 2000 microns.
Figure 3. Rotomolded products in this photo range from 55-gallon drums to billiard balls
Typical rotational molding applicationsRotational molding permits production of a countless number of fully or partially closed items. Design versatility of rotationally molded pieces is almost unlimited. The rigidity or flexibility of an item is controlled by the properties of the resin used (see section on Resin Choice) and by the wall thickness of the molding. Some typical applications for which rotational molding is particularly suited include the following: commercial, industrial and agricultural storage tanks ranging in size from 5 gallons to 22,000 gallons; containers for packaging and material handling; a variety of industrial parts, especially covers and housings, water softening tanks, tote bins; numerous under-the-hood and in-the-cab automotive parts; hobby horses, pool tables and many other small or large toys with complex shapes; baby cribs, balls, dolls, and doll parts; display window mannequins and other hollow display figures of all sizes, and; playground equipment and sporting equipment such as golf carts, footballs, juggling pins, helmets, dumbbells, golf tee markers, canoes and kayaks. Rotomolded parts are also used in portable outhouses, battery cases, light globes, vacuum cleaner and scrubber housings and garbage containers. Furniture, game housings, surf boards, traffic barricades, display cases and ducting can also be produced by rotomolding. The list above indicates just some of the possibilities. Figures 1-4 illustrate some of these applications.
Advantages of rotational moldingRotational molding offers significant advantages when compared with other molding techniques or thermoforming: costs for molds and tooling are relatively low; the rotomolding technique is easily adapted to short production runs, particularly when sets of multiple-cavity molds are used; hollow, totally enclosed items as well as pieces with openings can be made; rotational molding eliminates the need for secondary tooling; there is little or no waste due to resin scrap; wall thickness and piece weight can be easily controlled; rotational molding procedures assure uniform wall thickness; deviations can be controlled to within a maximum tolerance of 10 percent; pieces with intricate contours and undercuts can be easily molded; virtually any size piece can be rotationally molded; there is a minimum of crosssectional deformation and warpage; rotational molding yields pieces with excellent surface detail and finish; rotationally molded items are virtually stress free; identical or similar items or different sections on one piece can be molded at the same time in different colors on a single spindle; plastic or metal inserts can often be molded as integral parts of the item; and double wall constructions are feasible.
Design almost endless potentialWith rotomolding, a plastics product designer can create a huge array of innovative products. Typical design concerns that are handled routinely by rotational molding include the following: maintaining uniform wall thickness rotational molding can provide a more consistently uniform wall thickness for a part compared to other plastic processing methods; producing double-wall construction rotational molding can provide uniform double-wall construction on parts; molding thicker corners due to the process, rotomolded parts will have thicker outer corners which help strengthen the parts; and molding inserts, reinforcing ribs, kiss-off ribbing and undercuts these are easily included in a roto-molded part. Designers interested in acquiring more specific information can contact the Association of Rotational Molders, 2000 Spring Road, Oakbrook IL 60521, (630) 571-0611.
Figure 4. Large storage tanks are a major market for rotomolding
The Race Car Bed is rotationally molded from tough, scratch-resistant, high impact strength linear low density polyethylene.
Kids are all over this seven-foothigh Big Climber gym rotomolded from weather-resistant polyethylene. The colors have been molded-in, so the parts will not chip, splinter, rust or peel.
This rocking horse comes as either a palomino or a mustang. Both are rotationally molded from polyethylene.
The spinal immobilizer board used by emergency medical services has a rotomolded, linear medium density polyethylene, outer skin and a rigid urethane foam core.
Resin choiceTo obtain the desired end product, the choice of a quality powdered resin is essential in rotational molding. One reason is the high temperatures used risk chemical degradation in a less-than-quality product.Table 1. Usage of various resins for rotational moldingRESIN PERCENT OF MARKET 84%
Melt IndexFor rotomolding, a resin must have a good flow when molten. With polyethylene, the flow is measured by melt index. The higher the melt index, the better the flow. Most rotomolding resins have melt indices ranging from 2g/10 minutes to 10g/10 minutes. The term g/10 minutes refers to the weight of molten resin moving through an orifice of a predetermined size in 10 minutes. The melt index is also a rough measure of the molecular weight or the chain length of a resin. A resin with a high melt index has shorter chains and a lower molecular weight or smaller molecules. A resin with a low melt index has longer chains and a higher molecular weight or larger molecules. Molecular weight distribution is also important in a rotomolding resin. A narrow distribution is more advantageous, since the narrower the distribution, the more uniform the melt properties.
Polyethylene Polycarbonate Nylon Polyvinyl Chloride Polyesters Polypropylene ABS Acetals Acrylics Cellulosics Epoxy Fluorocarbons Phenolics Polybutylene Polystyrene Polyurethane Silicone
Type I: Low Density Resins (range of 0.925 g/cm3 and below). Generally, low density resins are preferable whenever stiffness is not essential or is undesirable, as for many toys, and only when light loads are to be expected. Type II: Medium Density Resins (range from 0.926 g/cm3 to 0.940 g/cm3). Most linear low density polyethylene resins fall within this range. Medium density resins are useful for selfsupporting items that require the higher heat-distortion resistance or stiffness that low density resins do not provide. Type III: High Density Resins (range from 0.941 g/cm3 to 0.959 g/cm3). High density resins impart the highest rigidity to the end product, which frequently permits reduction in wall thickness. Type IV: Very High Density Resins (0.960 g/cm3 and above.) These resins are not currently used i